Share this document with a friend

7

Transcript

HAL Id: hal-01090069https://hal.archives-ouvertes.fr/hal-01090069

Preprint submitted on 2 Dec 2014

HAL is a multi-disciplinary open accessarchive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come fromteaching and research institutions in France orabroad, or from public or private research centers.

L’archive ouverte pluridisciplinaire HAL, estdestinée au dépôt et à la diffusion de documentsscientifiques de niveau recherche, publiés ou non,émanant des établissements d’enseignement et derecherche français ou étrangers, des laboratoirespublics ou privés.

Proximity-Effect Driven Reversibility inSuperconducting Constrictions

Nikhil Kumar, Thierry Fournier, Hervé Courtois, Clemens Winkelmann, A.Gupta

To cite this version:Nikhil Kumar, Thierry Fournier, Hervé Courtois, Clemens Winkelmann, A. Gupta. Proximity-EffectDriven Reversibility in Superconducting Constrictions. 2014. hal-01090069

arX

iv:1

411.

7196

v1 [

cond

-mat

.sup

r-co

n] 2

6 N

ov 2

014

Proximity-Effect Driven Reversibility in Superconducting Constrictions

Nikhil Kumar,1 T. Fournier,2, 3 H. Courtois,2, 3 C. B. Winkelmann,2, 3 and Anjan K. Gupta1

1Department of Physics, Indian Institute of Technology Kanpur, Kanpur 208016, India2Universite Grenoble Alpes, Institut Neel, F-38042 Grenoble, France

3CNRS, Institut Neel, F-38042 Grenoble, France

(Dated: November 27, 2014)

We demonstrate the role of proximity effect in the thermal hysteresis of superconducting con-strictions. From the analysis of successive thermal instabilities in the transport characteristics ofmicron-size superconducting quantum interference devices with a well-controlled geometry, we ob-tain a complete picture of the different thermal regimes. These determine whether the junctions arehysteretic or not. Below the superconductor critical temperature, the critical current switches froma classical weak-link behavior to one driven by the proximity effect. The associated small amplitudeof the critical current makes it robust with respect to the heat generation by phase-slips, leading toa non-hysteretic behavior.

Micron-size superconducting quantum interference de-vices (µ-SQUID), consisting of two parallel weak links(WLs) acting as Josephson junctions in a small super-conducting (SC) loop, have been of interest for probingmagnetism at small scales [1–4]. One of the major obsta-cles of a µ-SQUID proper operation is its hysteretic (orbistable) current-voltage characteristic (IVC). When thecurrent is ramped up, it switches to a dissipative stateat the critical current Ic. When the current is rampeddown from above Ic, it comes back to a zero-voltage stateat a smaller current, called the re-trapping current Ir.In conventional tunnel-barrier type Josephson-junctions,the hysteresis arises from large junction capacitance [5].In WLs or µ-SQUIDs, with negligible capacitance, hys-teresis is found at low temperatures below a crossovertemperature Th < Tc [6], with Tc as the SC critical tem-perature. Although it has been claimed that an effectivecapacitance can arise from the recovery time of the SCorder parameter [7], it is now understood that hysteresisin WLs is of thermal origin [9–11], similar to that ob-served in superconductor-normal metal-superconductorjunctions [8]. Thermal hysteresis in SC-WLs and howit affects the IVCs can be modeled by considering lo-cal thermal balance which dictates the position of thenormal metal-superconductor (N-S) interface [9–11]. Incase of poor heat evacuation, phase fluctuations can trig-ger a thermal run-away giving a large resistive hot-spot.This topic is of great practical importance, in particu-lar for SC-magnet wires and cables, helium level sen-sors, bolometers [12], µ-SQUIDs and other nano-scale SCstructures [13]. A systematic understanding of variousthermal phases which a typical device exhibits is muchdesired, in particular to make devices with intrinsic non-hysteretic behavior.

In this Letter, we report on the transport characteris-tics of Nb-film based µ-SQUIDs with a well-controlledgeometry and describe a complete picture of differentthermal regimes. The IVCs show a critical current andtwo re-trapping currents that we describe using a ther-mal instability model in SC leads. The critical current

0 100 2000

100

200

300(b)

R (Ω

)

T (K)

7.5 8.0 8.5 9.00

40

80

120

Tc1

(c)

R (Ω

)

T (K)

Tc2

60 µ

m

2 µm

V+

V-

I+

I-(a)

FIG. 1: (a) SEM image of the µ-SQUID µS1 with its currentand voltage leads. The zoomed-in image shows the SQUIDloop (with area 1×1 µm2) and the narrow leads. (b) Resis-tance vs temperature (R-T) plot. (c) Low-temperature por-tion of the R-T plot, showing multiple transitions, for µS1 ata bias current of 0.01 mA.

Ic follows the theoretical expectation at low temperaturebut changes its behavior while crossing the smaller re-trapping current. In this hysteresis-free regime, the WLssuperconduct, despite being slightly heated by individualphase slips, thanks to the proximity effect of the adjacentsuperconductor.

We fabricated µ-SQUIDs from Nb films using commontechniques [2, 14–16]. After cleaning the Si substratewith an oxygen plasma, we deposited a 31 nm thick Nbfilm using e-beam evaporation in a UHV system. Wethen patterned the structures with electron beam lithog-raphy followed by deposition of a 20 nm thick Al film. Alift-off then transferred the pattern to the Al film, whichacts as a mask during the reactive ion etching of Nb usingSF6 plasma. Finally, the Al film was removed chemically.The transport measurements were carried out down to atemperature of 4.2 K in a home-made liquid helium dip-

2

per cryostat with built-in copper-powder filters [6]. Wehave studied more than four devices with similar behav-ior, but here we report on two typical devices denoted byµS1 and µS2.

For all devices, the patterned SQUID-loop area is 1µm2 and the width of its arms is 0.3 µm. The designedWL length is 150 nm while the WL width is 70 and 50nm in µS1 and µS2, respectively. Fig. 1(a) shows theSEM image of the device µS1. The pattern includes fourdifferent parts contributing to the electrical character-istics. The first part is the two WLs, each of normalresistance RWL. The second one is the SQUID loop withnormal resistance as RL including the resistance of theparallel WLs. The third part comprises the narrow leadsof width 0.3 µm and length 1.7 µm on either side of theSQUID loop, each with a resistance R1. Finally, each nar-row lead meets a wider lead of width 2 µm, length 27.5µm and normal resistance R2. From the geometry, var-ious resistances can be expressed in terms of the films’ssquare resistance R so that the total normal-state resis-tance between the voltage leads is RN = RL+2R1+2R2

= 40.3R+0.5RWL.

Figure 1(b) and (c) show temperature dependence ofthe four-probe resistance R for µS1. Multiple supercon-ducting transitions are observed. The resistance jumpsfrom its residual value 128 Ω down to about 40 Ω at Tc2

= 8.7 K, jumps further down from 38 to 8 Ω at Tc1 = 8.35K, and finally decreases smoothly to zero. We attributethe first transition at Tc2 to the wide leads, the secondone at Tc1 to both the narrow leads and the SQUID loop.From IVC in non-hysteretic regime, discussed later [seeFig. 3(f)], we deduce RWL ≃ 8 Ω. This analysis is consis-tent with R = 3.1 Ω, giving a resistivity of 9.5 µΩ.cm.

Next we discuss a one-dimensional model of thermalinstability in long current-biased SC leads. This is simi-lar to Broom and Rhoderick [17] model, which analyzesthe dynamics of an N-S interface under the influence of anelectrical current. Thus a critical magnitude of currentis found at which the N-S interface changes its directionof motion. Here we consider a SC lead with normal stateresistivity ρn, uniform thickness t and width w, and car-rying an electrical current I as shown in Fig. 2(a). Theheat transfer with the substrate at a bath temperatureTb writes α(T − Tb)/t, where the coefficient α is charac-teristic of the interface. The thermal conductivity κ isconstant and uniform. An N-S interface exists at x = 0,so that the temperature T is equal to Tc at this point.A heat current flows from x < 0 due to the resistance ofthis lead portion plus possibly a device at the end of thelead. With the boundary condition T = Tb at x → ∞,the heat equation solution in the SC portion of the leadis T = Tb + (Tc − Tb) exp(−x/lth). The thermal heal-ing length lth(=

√

κt/α) is a crossover length-scale suchthat for ∆x ≫ lth substrate heat-loss dominates and for∆x ≪ lth conduction dominates. The heat current at theN-S interface (x = 0) is then Q0 = wαlth(Tc−Tb), which

wt

x

z

y

I

x=0, T=Tc

TcTc+dT1 Tc-dT2

dxdx dx

normal superconducting

0Q&

0Q&

1Q&

T=Tb

x=0

(a)

(b)

FIG. 2: (a) Schematic of the semi-infinite (in +x direction)lead of SC material on a substrate at bath temperature Tb

with N-S interface at x = 0. (b) shows the region near the N-S interface with three differential elements of length dx whenthe N-S interface stabilizes near the heat source on left.

implies an effective thermal resistance of (wαlth)−1 as

seen from the N-S interface. It is important to realizethat the N-S interface will shift to the right (left) if more(less) than Q0 heat is incident on the lead at x = 0.For analyzing the stability of the N-S interface, we look

into the effect of fluctuations on a differential element(from x = 0 to x = dx) at this interface in a quasi-staticapproximation. If this element turns resistive, see Fig.2(b), an additional power I2ρndx/(wt) is generated. Thisextra heat is shared equally between the left and rightinterfaces to the lead, while the substrate receives a neg-ligible amount [18]. The heat current across the new N-Sinterface is Q′

1 = Q0 − α(Tc − Tb)wdx + I2ρndx/(2wt).As pointed out before, if this heat is more (less) than Q0,the N-S interface will shift to the right (left) implying in-stability (stability). Thus the maximum current that thelead can carry without causing a thermal instability isgiven by α(Tc − Tb)wdx = I2maxρndx/(2wt) or

Imax = w√

2α(Tc − Tb)/R. (1)

This expression is consistent with Ref. [9] results in thelimiting case of a very long SC lead and equal thermalconductivities of SC and normal metal, which is validclose to the N-S interface. In this model, the lead needsto be much longer than lth so that the overall thermalresistance as seen from the N-S interface does not dependon its position. When I exceeds Imax, the N-S interfacewill runaway to a large x location where the lead joinsa thermal bath (or a much wider lead) as the thermalresistance to the thermal bath will be less there. Byanalyzing the stability of a small resistive element againstan incursion to the SC state, one finds as expected thesame expression for the re-trapping current. It would bemore appropriate to call Imax as the ‘instability current’as it describes both the runaway and re-trapping of theN-S interface. We will use the term ‘re-trapping’ current,

3

as it has been done in most earlier works.

In order to quantify in our case the relevant parame-ters, we use the Wiedemann-Franz law to estimate thethermal conductivity as κ = LT/ρ with L = 2.44×10−8

W.Ω/K2 as the Lorenz number. Using T = Tc = 8.5 Kand ρ = 9.5 µΩ.cm, we get κ = 2.4 W/cm.K. Typicalvalues of α that have been used in literature [9, 11] rangein 1 to 10 W/cm2.K. We use α = 5.3 W/cm2.K as foundfrom the temperature dependence of a re-trapping cur-rent as discussed later. From these values, we estimatethe thermal healing length for our devices as lth = 1.6µm. The length of the wide leads, i.e. 27.5 µm, is thusmuch longer than lth while that of the narrow leads, i.e.1.7 µm, is only comparable to lth.

Fig. 3 shows IVCs of µS1, depicting sharp jumps involtage at three different currents, namely Ir1, Ir2 andIc. The critical current Ic is defined by the first jumpseen while ramping the current up from zero. It showsa distribution of values with, for µS1, a width of about40 µA for a mean value of 1.3 mA at 4.2 K [18]. Fromthe IVC slope, the resistance just above Ir1 is about 48Ω. This value is close to the sum RL+2R1 = 40 Ω ofthe resistances of the SQUID loop and the narrow leads,which means that the latter are heated to above Tc forI > Ir1. The observed extra resistance indicates that aportion of the wide leads is also heated to above Tc, thuscontributing to the resistance. The second re-trappingcurrent Ir2 arises from a thermal instability in the longand wide leads. The IVC slope above Ir2 is 140 Ω, whichis close to the normal-state resistance value 128 Ω, in-dicating a thermal runaway till the voltage leads. Theslightly larger value seen here is due to the heating inthe central portion to more than 50 K as estimated froma thermal model. At higher temperatures when Ir2 ismuch less and thus the heating is also reduced, the re-sistance above Ir2 is found to be exactly 128 Ω. In thisregime, Fig. 3(f) shows that the resistance just above Icis about 4 Ω from which we deduce RWL as 8 Ω. Only thecritical current Ic was found to oscillate with the mag-netic flux [18] as expected for a SQUID. The retrappingcurrents Ir1,2 do not, which confirms that they are notdependent on the SC of the WL.

The three currents Ir1, Ir2 and Ic evolve differentlywith temperature. Near 5.7 K, Ic crosses Ir2 [see Fig.3(b)] and at T = Th = 7.25K, Ic crosses Ir1 [see Fig.3(e)], so that hysteresis is absent at higher temperature[see Fig. 3(f)]. We observe sharp voltage changes corre-sponding to the three currents, making them distinguish-able from each other. With increasing temperature, whilethe IVC near Ic becomes relatively smooth, the voltagejump corresponding to Ir1 remains sharp and evolves overthis smooth feature. Also, the hysteresis does not dis-appear untill Ir1 fully crosses this smooth feature [seeFig.3(e)]. This confirms that the two transitions havedistinct origins.

Figure 4(a) summarizes the bath-temperature depen-

0.0 0.2 0.40

204060 T = 7.25 K

V

(mV

)

I (mA)

Ic, Ir1Ir2

0.00 0.05 0.10 0.15 0.200

2

4

6

8

Ir1

Ic

(e)

V (m

V)

I (mA)0.00 0.05 0.10 0.150

2

4

6 Ir1

Ic

(f)

V (m

V)

I (mA)

T = 7.65K

0.0 0.2 0.4 0.60

25

50

75

Ir1 Ir2

IcT = 5.73 K

(b)

V (m

V)

I (mA)0.0 0.4 0.8 1.20

50

100

150

Ir1

Ir2

IcT = 4.25 K

V (m

V)

I (mA)

(a)

0.0 0.1 0.2 0.3 0.4 0.50

20

40

60

Ic

Ir2Ir1

T = 7.0 K

(d)

V (m

V)

I (mA)0.0 0.2 0.4 0.60

20

40

60

80

Ir2Ir1

Ic

T = 6.27 K

(c)

V (m

V)

I (mA)

FIG. 3: (a) - (d) IVCs in hysteretic regime for µS1 at differenttemperatures. A large hysteresis is seen at 4.25 K with twore-trapping currents, Ir1 and Ir2. Ic crosses Ir2 near 5.7 Kand Ir1 around 7.25 K as seen in (e). (f) shows the IVC ofµS1 in the non-hysteretic regime above Th = 7.25 K. Theinset of (e) shows a larger bias-current range plot to show theIr2 transition.

dence of Ic, Ir1 and Ir2 for µS1. Fig. 4(b) shows the samefor the device µS2, which has narrower WLs as comparedto µS1, leading to a smaller critical current, and thus asmaller crossover temperature and a wider temperaturerange of non-hysteretic IVCs. The retrapping currentsIr1,2 are the same in the two samples, which confirmsthat these are independent of the WL structure. Withincreasing bath temperature, the critical current Ic de-creases linearly in both devices up to Th, where it showsa marked change in behavior. For both devices, Ic andIr1 go to zero at the temperature Tc1, while Ir2 van-ishes at Tc2. This is consistent with the R-T behaviorof Fig. 1(c) for µS1. In both plots, we also indicate thestate (resistive or SC) of different portions of the devicewhen the current is ramped down, which constitutes akind of a phase diagram, or more appropriately, statediagram. The light gray-shaded area shows the bistableregion where the whole device is in the fully SC stateduring the current ramp-up from zero. In the dark gray-shaded region, only the WLs are resistive. No hystere-sis is observed in the related temperature range [Th,Tc1].This is the most desirable mode for a SQUID, but it oc-curs in quite a limited temperature window. At a fixed

4

4.5 5.0 5.5 6.0 6.5 7.0 7.5 8.0 8.50.0

0.2

0.4

0.6

0.8

ThTc1

Tc2

S2(b)

Ic

Ir1Ir2

Cur

rent

(mA

)

Bath Temp (K)

0.0

0.2

0.4

0.6

0.8

1.0

1.2

(a) S1Tc1

Tc2

Th

Ir2

Ir1

Ic

Cur

rent

(mA

)

FIG. 4: Variation of Ic, Ir1 and Ir2 with bath temperaturefor (a) µS1 and (b) µS2. The symbols are the data points.The continuous lines are fits given by (in mA and K), (a)Ic = 0.42(7.4 − Tb) and (b) Ic = 0.29(7.4 − Tb) while theother two are described by Ir1 = 0.17(8.4− Tb)

0.43 and Ir2 =0.37(8.7 − Tb)

0.5 for both the devices. The cartoon picturesof the device shown in different regions depict the state ofthe device during current ramp-down with blue as SC andred as resistive portions. The light gray-shaded area showsthe bistable region where the whole device is in the fully SCstate during the current ramp-up from zero. In the dark gray-shaded region, only WLs are resistive.

current bias, we do see the expected voltage oscillationswith flux in this regime [18].

Using the long lead approximation for the wide leads,we can fit Ir2 with Eq. 1 which writes here Ir2 =w√

2α(Tc2 − Tb)/R. We obtain a very good fit, see Fig.4 with the only free parameter being α = 5.3 W/cm2.K,in good agreement with reported values [9, 11]. Withthe same parameters, except w = 0.3 µm, Eq. 1 predictsfor the narrow leads a current Ir1 significantly smallerthan observed. This is expected as the presence of wideleads at a short distance makes the heat evacuation moreefficient, leading to a higher run-away current.

In a short WL, i.e. with dimensions less than the SCcoherence length, we expect, close to its critical temper-ature, a linear decrease of Ic with temperature so that

IcRWL = β(Tc − Tb) with β = 0.635 mV/K [3]. Fromthe Ic slope in Fig. 4(a) for µS1 at temperatures belowTh, we find a RWL/2 value of 3 Ω, which agrees withour earlier findings. In this same regime, the extrapo-lated critical temperature value of 7.4 K is related to theintrinsic superconductivity of the WLs. Above Th, thetemperature dependence of Ic changes slope and goesdown to zero precisely at the critical temperature Tc1

of the SQUID loop. From this observation, we concludethat the WLs are SC above Th owing to proximity effectfrom the adjacent SC with a higher critical temperature.

Finally, we elaborate on how the behavior change ofIc coincides with its crossing with Ir1 at Th. Below thecrossover temperature Th, the critical current Ic exceedsthe stability (retrapping) current Ir1. In this case, a sin-gle phase-slip event induced by thermal fluctuations inthe WL can cause a thermal runaway [13]. IVCs thusexhibit a sharp voltage jump at Ic, see Fig. 3(a-d). Adistribution of Ic values is obtained, since a phase slip-induced transition is stochastic [20]. Above the crossovertemperature Th, the critical current Ic is smaller thanthe stability (runaway) current Ir1, so that no thermalrunaway can happen at Ic: the reversible (mono-stable)regime is obtained. Due to phase-slips proliferation nearIc, the transition to the resistive state (at Ic) is thensmeared, see Fig. 3(e). The related non-zero dissipa-tion just below Ic also heats some portion of the deviceabove the bath temperature Tb. Assuming that the wholeSQUID loop is at nearly uniform temperature, which isjustified since the loop size is comparable to lth, we es-timate that the power generated just below Ic of 72 nWfor Tb = 7.25 K brings the SQUID loop to a temperatureof about 7.8 K. Because of this and of the fact that theWL region is actually a SC with a lower critical temper-ature, the temperature dependence of Ic between Th andTc1 cannot be simply described by that of S-N-S WLs[19]. Due to their respective temperature dependence, Icand Ir1 are expected to cross at some temperature evenif the WL Tc is same as that of the adjacent SC. But thenthe hysteresis-free regime would have existed over a muchnarrower temperature range. Thus the smaller Tc of theWL and the proximity SC plays crucial role in wideningthis hysteresis-free temperature range. Finally, SQUIDdevices with lower Ic or higher Ir1 values will help widenthis temperature range even further.

In conclusion, we present the complete device-statediagram of Nb based µ-SQUIDS. We highlight a non-classical weak link behavior which is understood in theframework of a thermal instability picture. The non-hysteretic high temperature regime of the weak-links isshown to benefit from proximity superconductivity. Thepresent new understanding of the physical mechanisms atthe origin of a non-hysteretic behavior is key to furtherdevelopments in µ-SQUID magneto-sensors for which thesuppression of hysteresis represents a key issue.

Samples were fabricated at the platform Nanofab,

5

CNRS Grenoble and measurements were carried out inIIT Kanpur. AKG thanks University Joseph Fourierfor a visiting fellowship. NK acknowledges the finan-cial support from CSIR, India. This work has been fi-nanced by the French Research National Agency, ANR-NanoQuartet (ANR12BS1000701) and the CSIR of thegovt. of India.

[1] W. Wernsdorfer, Adv. Chem. Phys. 118, 99 (2001).[2] K. Hasselbach, C. Veauvy, D. Mailly, Physica C 332, 140

(2000).[3] K. K. Likharev, Rev. Mod. Phys. 51, 101 (1979).[4] D. Hazra, J. R. Kirtley, and K. Hasselbach, Appl. Phys.

Lett. 103, 093109 (2013).[5] M. Tinkham, Introduction to Superconductivity 2nd ed.

(Mc Graw-Hill, New York, 1996).[6] D. Hazra, Hysteresis in superconducting weak links and

micron size superconducting interference devices, PhDthesis, IIT Kanpur (2011).

[7] Y. Song, J. Appl. Phys. 47, 2651 (1976); S. Michotte, S.Matefi-Tempfli, L. Piraux, D. Y. Vodolazov and F. M.Peeters, Phys. Rev. B 69, 094512 (2004).

[8] H. Courtois, M. Meschke, J. T. Peltonen, and J. P.Pekola, Phys. Rev. Lett. 101, 067002 (2008).

[9] W. J. Skocpol, M. R. Beasley, and M. Tinkham, J. Appl.Phys. 45, 4054 (1974).

[10] M. Tinkham, J. U. Free, C. N. Lau, and N. Markovic,Phys. Rev. B 68, 134515 (2003).

[11] D. Hazra, L. M. A. Pascal, H. Courtois, and A. K. Gupta,Phys. Rev. B 82, 184530 (2010).

[12] K. S. Ilin, M. Lindgren, M. Currie, A. D. Semenov, G.N. Goltsman, R. Sobolewski, S. I. Cherednichenko andE. M. Gershenzon, Appl. Phys. Lett. 76 , 2752 (2000).

[13] N. Shah, D. Pekker, and P. M. Goldbart, Phys. Rev. Lett101, 207001 (2008).

[14] L. Angers, F. Chiodi, G. Montambaux, M. Ferrier, S.Gueron, H. Bouchiat, and J. C. Cuevas, Phys. Rev. B77, 165408 (2008).

[15] S. K. H. Lam and D. L. Tilbrook, Appl. Phys. Lett. 82,1078 (2003).

[16] Nikhil Kumar, T. Fournier, H. Courtois, and Anjan K.Gupta, AIP Conference Proceedings 1591, 1591 (2014).

[17] R. F. Broom and E. H. Rhoderick, Brit. J. Appl. Phys.J. Phys. 11, 292 (1960).

[18] See the supplementary Information below.[19] P. Dubos, H. Courtois, B. Pannetier, F. K. Wilhelm, A.

D. Zaikin, and G. Schon, Phys. Rev. B 63, 064502 (2001).[20] T. A. Fulton and L. N. Dunkelberger, Phys. Rev. B 9,

4760 (1974).

Supplementary Information

SQUID oscillations with magnetic flux

Figure 5 below shows the oscillations in Ic for µS1 at4.25 K (below Th) and in voltage at 7.4 K (above Th)with external magnetic flux. The voltage oscillations are

0 1 2 3 40.4

0.6

0.8

1.0

1.2

1.4

V (T = 7.4K)

I c(m

A) ,

V (m

V)

B (mT)

Ic(T = 4.25K)

FIG. 5: Ic oscillations in hysteretic regime for µS1 at 4.25K(Red curve) and the voltage oscillations (at 0.17mA current)in non-hysteretic regime at 7.4K (Blue curve).

acquired at a bias current of 0.17 mA, which is close tothe critical current at this 7.4 K. The SQUID oscillationswith magnetic field are seen only in Ic and not in Ir1and Ir2. The temperature dependent Ic values have beenextracted from these Ic-Vs-B plots at all temperatures byselecting maximum Ic at each temperature. In the non-hysteretic regime Ic was found from the maximum slopeof the IVC. This is found to coincides with the currentat which the voltage modulation in V-Vs-B peaks. Inboth cases, the magnetic field periodicity is found to be1.5 mT, which defines an effective SQUID loop area asAeff = φ0

∆B= 1.3µm2, which is larger than the actual

patterned (internal) area of 1 µm2.

Heat sharing during resistive fluctuation

In order to elaborate on the sharing of the extra re-sistive heat, when the differential element becomes nor-mal, by the three interfaces, we also consider two neigh-boring differential elements of the same length dx asshown in Fig. 2(b) of the main paper. The one on theleft (i.e. from x = −dx to x = 0) is at temperatureTc + dT1 and the one on the right (i.e. from x = dx tox = 2dx) is at temperature Tc − dT2. The left one givesheat Q0 = κwtdT1

dxto the middle one, which gives heat

Q1 = κwtdT2

dxto the element on right and thus we get,

κwtdT1

dx= α(Tc − Tb)wdx + κwt

dT2

dx(2)

When the middle element becomes resistive due to fluc-tuations its temperature increases to Tc + dT . In this

6

case the above equation gets modified to

κwtdT1 − dT

dx= α(Tc + dT − Tb)wdx

+ κwtdT2 + dT

dx− I2

ρnwt

dx (3)

Subtracting eq. 2 from eq. 3 we get 2κwtdTdx

= I2 ρndxwt

−

αdTwdx. Neglecting the higher order second term on the

right, we get κwtdTdx

= I2 ρndx2wt

. Thus the heat current

incident from the left interface, i.e. Q′

0 = κwtdT1−dTdx

=

Q0 − I2 ρndx2wt

and the heat current incident at the right

interface, i.e. Q′

1 = κwtdT2+dTdx

= Q1 + I2 ρndx2wt

. Thusthe extra heat generated is equally shared across the twointerfaces.

Recommended